Single-Molecule Tracking of Polymer Surface Diﬀusion Michael J. Skaug, Joshua N. Mabry, and Daniel K. Schwartz* Department of Chemical and Biological Engineering, University of Colorado Boulder, Boulder, Colorado 80309, United States S Supporting Information *

ABSTRACT: The dynamics of polymers adsorbed to a solid surface are important in thin-ﬁlm formation, adhesion phenomena, and biosensing applications, but they are still poorly understood. Here we present tracking data that follow the dynamics of isolated poly(ethylene glycol) chains adsorbed at a hydrophobic solid−liquid interface. We found that molecules moved on the surface via a continuous-time random walk mechanism, where periods of immobilization were punctuated by desorption-mediated jumps. The dependence of the surface mobility on molecular weight (2, 5, 10, 20, and 40 kg/mol were investigated) suggested that surface-adsorbed polymers maintained eﬀectively three-dimensional surface conformations. These results indicate that polymer surface diﬀusion, rather than occurring in the two dimensions of the interface, is dominated by a threedimensional mechanism that leads to large surface displacements and signiﬁcant bulk−surface coupling.

■

INTRODUCTION In lubrication1 and adhesion phenomena,2 at biointerfaces, and in thin-ﬁlm formation processes,3 polymer molecules adsorb to a solid surface,4 and their dynamics govern subsequent relaxation and transport. While the motion of polymers in the “melted” state or in solution is fairly well understood,5 the mechanisms by which polymers move on surfaces remain mysterious and a matter of debate.6−12 It is clear, however, that polymer dynamics are signiﬁcantly slowed near an attractive interface.4,13 For example, surface diﬀusion coeﬃcients are often orders of magnitude lower than bulk values,4,14 but the available experimental evidence does not conclusively identify a dominant mechanism of polymer surface diﬀusion and suggests that the mechanism may depend on the surface and the chain length.9,10 Part of the diﬃculty in understanding polymer surface dynamics is that polymer surface conformations may be diﬀerent than bulk conformations and can vary depending on the polymer−surface interaction, the chain length, and surface coverage.13 The conventional picture is that polymers adsorb to a solid surface with a “loop−train−tail” conformation in which adsorbed chain segments are “trains” separated by “loops” of unabsorbed monomers.13 The bound fraction (the fraction of polymer segments adsorbed in trains) is one measure of the adsorbed chain conformation. The equilibrium bound fraction is predicted to depend on the monomer−surface interaction energy, χs, and the chain length, N. For short chains (N < 10) or strongly adsorbing monomers (χs > 1kT), the bound fraction approaches unity, while for longer chains or weakly attractive monomers, the bound fraction is typically in the range 0.5 to 1.6,15 Previous experiments have found bound fractions between 0.5 and 0.75 for polymers adsorbed at low surface coverage, suggesting a ﬂattened two-dimensional conformation.9,16 However, this picture is further complicated if adsorbed chains relax toward equilibrium very slowly.17,18 Whether an adsorbed chain is strictly two-dimensional or in a more three-dimensional © 2013 American Chemical Society

conformation has a signiﬁcant inﬂuence on the possible mechanism by which a polymer moves across a surface. To uncover the detailed mechanism of polymer surface diffusion, we conducted a series of single-molecule tracking experiments to probe the behavior of isolated linear homopolymer chains at a hydrophobic solid−aqueous interface. Speciﬁcally, we studied a series of poly(ethylene glycol) (PEG) chains whose molecular weight varied by more than an order of magnitude. The primary driving force for PEG adsorption to the solid surface was the hydrophobic interaction.9,19 Because the hydrophobic interaction is nonspeciﬁc and relatively long-ranged compared with other intermolecular forces, the system we studied represents the case of a delocalized, long-range polymer−surface interaction. We observed polymer surface transport characterized by desorption-mediated displacements that were interrupted by periods of immobility, qualitatively similar to a previous report for the surface diﬀusion of other molecular species.20 A desorption-mediated surface displacement is one where, instead of moving in the plane of the surface, the molecule desorbs, diﬀuses in the bulk liquid, and readsorbs at a new surface location. A speciﬁc example of a continuous-time random walk,21 this mechanism can be described as “intermittent hopping” because each desorption-mediated surface displacement is separated by a random period of apparent surface immobilization. One consequence of the desorption-mediated mechanism is that large displacements are much more probable than if the process involved normal (Gaussian) Brownian motion within the plane of the surface. The prevalence of large surface displacements and the intermittency of the trajectories are predicted to dramatically inﬂuence the rate at which a polymer ﬁnds a surface target,22,23 a key process in heterogeneous catalysis, biosensing, and other Received: July 18, 2013 Published: November 10, 2013 1327

dx.doi.org/10.1021/ja407396v | J. Am. Chem. Soc. 2014, 136, 1327−1332

Journal of the American Chemical Society

Article

ﬂuctuations, taken from the distribution f vib(r) = [l(2π)1/2]−1 exp(−r2/ 2l2) with l = 0.04 μm, were added to the molecular position to account for apparent motion due to experimental localization uncertainty. After each random waiting time, a random surface displacement was selected using eq 1. The constant r* = D/(Qadsb) contains three parameters, but the bulk diﬀusion coeﬃcient D and the radius of gyration b can be set to known or independently calculated values, leaving Qads as the only free parameter used in the simulations to match the experimental results. The complete set of simulation parameters are provided in Table S1 in the Supporting Information. The diﬀusion coeﬃcients were taken from the literature,26 and the radius of gyration was calculated using b = aN3/5, where a = 0.35 nm is the PEG monomer size.27

technologies. Our results also highlight the fact that surface diﬀusion is not necessarily a two-dimensional process but is coupled to three-dimensional motion near the surface, potentially making surface diﬀusion sensitive to the near-surface liquid environment. In fact, our observations imply strong bulk−surface coupling, where the average diﬀusion of polymers well away from the surface is reduced.14

■

EXPERIMENTAL SECTION

Single-Molecule Tracking. We used total internal reﬂection ﬂuorescence microscopy (TIRFM)20 to track the motion of individual polymer chains at a planar interface between aqueous solution and polished fused silica coated with a hydrophobic trimethylsilyl (TMS) monolayer.24 We collected image sequences of ﬂuorescently labeled polymers as they randomly adsorbed and moved on the surface at dilute surface coverage. Using custom image analysis in Mathematica, we identiﬁed the positions of the polymers in each image and extracted molecular surface trajectories from the image sequences (Figure 1a). The polymer chains were PEG of nominal molecular weights 2, 5, 10, 20, and 40 kg/mol, corresponding to N = 45, 113, 227, 454, and 908 monomer units. The polymer was end-labeled with ﬂuorescein isothiocyanate (PEG, Nanocs, USA). The PEG samples were dissolved at low concentration (10 fM to 600 pM) in 1 mM sodium borate buﬀer at pH 8.6 and injected into a custom ﬂow cell and imaged as previously described.24 In a control experiment, we found that ﬂuorescein isothiocyanate does not adsorb appreciably to the surface at the concentrations used in this study, indicating that the PEG−surface interaction was the dominant driving force for polymer surface adsorption. We estimate that the PEG monomer−surface interaction energy in our experiments was similar to the value of ∼0.5kT measured on a similar hydrophobic surface.9 The bulk concentrations were selected such that the surface coverage was approximately 0.01 molecule/μm2 (∼10−3 mg/m2), meaning that the measurements were made in the dilute limit where no polymer−polymer interactions were expected. Although the degree of labeling was not veriﬁed, a small amount of unlabeled polymer would not be expected to inﬂuence the dynamics at such dilute concentrations. Image sequences of polymer adsorption, diﬀusion, and desorption were recorded with an exposure time of 0.05 or 0.1 s. Because of their fast diﬀusion (D > 10 μm2/s) in solution, molecules could be identiﬁed and tracked only when they were adsorbed to the solid surface. Trajectories were constructed by connecting nearest-neighbor objects in consecutive frames given a maximum allowed displacement of Rmax = 2.2 μm. The possibility of falsely connecting two molecules into a single trajectory was recently discussed,20 and all of the results are based on trajectories that lasted more than 2 s. Simulations. To simulate molecular surface trajectories, we used a model similar to one that was previously described,20 except that the desorption-mediated surface displacements were drawn from the recently published exact expression for W(r), the distribution of individual surface displacements produced by excursions through the bulk liquid:25

W (r ) =

⎛ r ⎞⎤ 1 1 ⎡ ⎜⎛ r ⎟⎞ − − Y0⎜ ⎟⎥ H0 2⎢ ⎝ ⎠ ⎝ r * ⎠⎦ 2πr(r*) r* 4(r*) ⎣

■

RESULTS In analyzing the motion of individual polymer chains as they moved at the interface between a buﬀer solution and a hydrophobic substrate, a notable qualitative observation involved the signiﬁcant heterogeneity between molecular trajectories (Figure 1b).

Figure 1. Intermittent-hopping mechanism of polymer surface diﬀusion. (a) Experimental ﬂuorescence images of a 40 kg/mol PEG polymer moving at the solid−liquid interface. The scale bar represents 1.0 μm. (b) Representative trajectories of 40 kg/mol polymers that illustrate the intermittent nature of the dynamics. For comparison, a normal random walk (generated via a computer simulation) with the same eﬀective diﬀusion coeﬃcient as the experimental trajectories is depicted in magenta. (c) Data for the 40 kg/mol polymer showing lateral position as a function of time to highlight the periods of immobility. (d) Illustration of the proposed desorption-mediated mechanism governing polymer surface diﬀusion.

(1)

where H0 is the Struve function, Y0 is a Bessel function of the second kind, and the parameter r* = D/(Qadsb) incorporates the fundamental physical parameters of the system: the bulk diﬀusion coeﬃcient D, the adsorption rate constant Qads, and the polymer radius of gyration b. Equation 1 is valid at time scales longer than a typical desorptionmediated displacement, which was the case in our experiments where displacements were eﬀectively instantaneous. The empirical waitingtime distributions ψ(τdes) were modeled using the expression

Some trajectories appeared to be completely immobile while others were mobile or displayed intermittent behavior. We also noted the occurrence of some very large displacements across the surface (Figure 1b). These two observations are qualitatively inconsistent with the behavior expected for a molecule diﬀusing via normal Brownian motion in two dimensions. The same qualitative behavior was observed for all of the molecular weights studied and was similar to the dynamics reported for the surface diﬀusion of other molecular species.20,28

⎡ ⎤⎛ 1 ⎞1 + α α1 − α ψ (τdes) = ⎢ ⎥⎜ ⎟ ⎣ τdes −α (α − 1)−α ⎦⎝ τdes ⎠ where α = 1.5 and the mean waiting time ⟨τdes⟩ were measured experimentally.20 During each period of immobilization, random spatial 1328

dx.doi.org/10.1021/ja407396v | J. Am. Chem. Soc. 2014, 136, 1327−1332

Journal of the American Chemical Society

Article

guide, we deﬁned a distance threshold of Δr = 0.2 μm to distinguish real surface displacements from apparent motion during immobilization. For all polymer chain lengths, we found that the periods of immobilization were characterized by the same approximately power-law distribution of waiting times, ψ(τdes) ∼ τdes−(1+α), where α = 1.5 (Figure 3). As one would

To quantify the polymer surface dynamics, we analyzed the distributions of molecular surface displacements (Figure 2) using the self-part of the van Hove correlation function,

Figure 2. Distributions of surface displacements. The symbols represent experimental data for PEG of diﬀerent molecular weights (as annotated) at the solid−liquid interface for a time interval Δt = 0.1 s. The solid lines are simulation results using the model described in the text. The dashed line is a Gaussian with the same eﬀective diﬀusion coeﬃcient as the 40 kg/mol data (D ≈ 0.075 μm2/s). The curves were shifted vertically to allow easier interpretation (the 2, 5, 10, 20, and 40 kg/mol data sets were shifted by factors of 3, 5, 0.5, 0.02, and 0.001, respectively).

Gs(Δx , Δt ) =

1 N

Figure 3. Distributions of the waiting time between desorptionmediated surface displacements. Symbols with connecting lines are the experimental data for PEG of diﬀerent molecular weight (as annotated). Curves were displaced vertically to allow easier interpretation (the 2, 5, 20, and 40 kg/mol data sets were shifted by factors of 1/15, 1/5, 5, and 15, respectively.) The dashed line illustrates the approximate τdes−2.5 behavior of the distributions.

N

∑ δ[Δx + xi(t ) − xi(t + Δt )]

intuitively expect, we found that the mean waiting time, ⟨τdes⟩, increased with increasing chain length. A theoretical prediction for this increase, based on equilibrium conﬁgurations of adsorbed chains, is that the mean desorption time should scale as eN, where N is the number of monomers.30 However, we observed powerlaw scaling of the mean desorption time: ⟨τdes⟩ ∼ Nβ, where β = 0.6 ± 0.1 (Figure 4a). The signiﬁcance of this exponent is discussed in more detail below. This ﬁnding was robust with respect to variations in the data analysis parameters. For example, changing the distance threshold used to deﬁne immobilization by ±0.04 μm resulted in a ±18% change in mean waiting time and little change in the approximate power-law exponent. Despite the non-Gaussian displacement distributions, we found that the mean-square displacement (MSD) increased approximately linearly with time (Figure 5). In the absence of the displacement distributions (Figure 2), this would be consistent with normal Brownian motion, that is, the MSD is insensitive to the detailed mechanism of surface diﬀusion, as has been previously observed.20,31 The roughly equal spacing between the MSD curves in Figure 5 suggests a power-law dependence of the transport coeﬃcient on chain length. To characterize this dependence in a way that allows comparison with previous reports, we calculated an ef fective surface diﬀusion coeﬃcient at short times, Deff, by ﬁtting the MSD to a linear model over the ﬁrst four data points. We found that Deff ∼ Nγ, where γ = −0.6 ± 0.2 (Figure 4b). As mentioned above, the non-Gaussian tails of the displacement distributions (Figure 2) are not consistent with a normal two-dimensional random walk. Interestingly, power-law-distributed displacements were predicted theoretically for interfacial molecular motion dominated by desorption-mediated diﬀusion.32 Desorption-mediated surface displacements occur when a molecule desorbs from the interface, begins diﬀusing in the adjacent three-dimensional bulk (liquid) phase, and readsorbs at a new location on the surface before being lost completely from the surface.25,32 In the standard model, this occurs under strongly adsorbing conditions deﬁned by the molecule’s surface

i=1

(2)

This distribution represents the probability that a molecule has moved a distance Δx along the x or y coordinate during time Δt. The two salient qualitative features of the measured displacement distributions are the narrow central peaks and the non-Gaussian tails (Figure 2). The tails of the distributions evolve from approximately exponential for the polymer with the lowest molecular weight to approximately power-law for the largest polymer (the non-Gaussian tails of the distributions are highlighted in Figure S1 in the Supporting Information). This contrasts with the Gaussian distribution that would be expected if the polymer chains were undergoing normal two-dimensional Brownian motion at the interface. Qualitatively, we observed the expected decrease in mobility with increasing molecular weight, as evidenced by the narrowing of the displacement distributions (Figure 2). However, as illustrated by the dashed line in Figure 2, a simple random-walk model for surface diﬀusion certainly does not describe the central peaks and non-Gaussian tails of the distributions. The narrow central peaks of the displacement distributions do not broaden with increasing lag time (Figure S2 in the Supporting Information), suggesting that they are associated with periods of immobility or conﬁnement.20 We believe that the ﬁnite width of the central peaks is primarily due to imperfect localization of molecules in the ﬂuorescence images.29 In fact, the width of the central peaks, σ ≈ 0.04 μm, is a measure of our experimental localization precision and implies that we were able to resolve only displacements much greater than the polymer coil size. Although there may have been conﬁned or slow diﬀusion (D < 0.002 μm2/s) during periods of apparent immobility, the molecules appeared immobilized given our experimental localization precision and trajectory lengths. The intermittency of the trajectories can be characterized statistically by the distribution of waiting times, τdes, between surface displacements. Using the displacement distributions as a 1329

dx.doi.org/10.1021/ja407396v | J. Am. Chem. Soc. 2014, 136, 1327−1332

Journal of the American Chemical Society

Article

Figure 2 with the predicted Cauchy distribution.25,32 However, the standard theoretical model assumes a single desorption time, which is inconsistent with the experimentally measured waitingtime distributions (Figure 3), which exhibited long tails. We therefore chose to simulate the molecular surface trajectories using the empirical waiting-time distributions (Figure 3) and the analytical expression for the distribution of single-desorptionmediated displacements W(r) (eq 1). Using Qads (the adsorption rate constant) as the only free parameter in the simulations, we found reasonable agreement with the experimental displacement distributions (Figure 2) when Qads decreased with increasing molecular weight (Figure 4c). In fact, we found the approximate scaling Qads ∼ Nδ, where δ = −1.2 ± 0.1. We note that the standard model for desorption-mediated diﬀusion, which assumes a single characteristic desorption time, predicts superdiﬀusive behavior in strongly adsorbing systems,25,32 yet the measured MSD was either Fickian or slightly subdiﬀusive (Figure 5). The most likely reason for this discrepancy is the existence of long periods of immobilization over the entire experimental time scale (Figure 1c), as opposed to a single characteristic desorption time.25,32

■

DISCUSSION Dependence of the Chain Dynamics on Molecular Weight. We observed polymer surface diﬀusion that was welldescribed by an intermittent-hopping mechanism. Moreover, the chain dynamics exhibited a clear and systematic dependence on the molecular weight. On the basis of statistical models of polymer chain conformations, it is possible to interpret this chain-length dependence to obtain additional information about polymer conformations and dynamics. In what follows, we examine the implications of the observed dynamic scaling and how it compares with previous ideas about polymer surface behavior. We start with the scaling of Qads, which can be rationalized in terms of p, the probability that the chain adsorbs during each surface encounter. The adsorption rate is Qads = p/τcoil, where τcoil = b2/D is the time that the polymer chain remains within a distance b of the surface (i.e., in contact with the surface) if it has a bulk diﬀusion coeﬃcient D. With the assumption that each monomer−surface interaction is identical, p ∼ Nν follows from the fact that the number of monomers in contact with the surface scales as Nν.9,13 Because b ∼ Nν and D ∼ N−ν for a polymer in dilute solution,5 it follows that Qads ∼ N−2ν. Assuming good solvent conditions for PEG in water (i.e., ν = 0.6) leads to the prediction that Qads ∼ N−1.2, as observed. The scaling discussed above also leads to a surprising prediction for equilibrium polymer adsorption, which was identiﬁed in earlier experiments.9 In adsorption isotherm measurements, the adsorption rate and desorption rate (or inverse mean waiting time ⟨τdes⟩−1) combine to give the slope of the isotherm, h = Qadsb/⟨τdes⟩−1. Using our previously outlined scaling theory for Qads and b and noting our empirical ﬁnding for the scaling of ⟨τdes⟩−1, we infer that h would be independent of the polymer molecular weight. This extrapolation from our single-molecule results is consistent with macroscopic adsorption measurements made on a similar experimental system consisting of PEG at a hydrophobic−water interface.9 Interestingly, these observations suggest that the diﬀerence between the diﬀusive behaviors of short and long chains is primarily due to the times of immobilization and not the step sizes during mobile periods. To see this, we note that the surface is modeled as an adsorptive sink of width b with strength

Figure 4. Chain length scaling of polymer surface dynamics and kinetics. (a, b) Plots of (a) the mean waiting time and (b) the eﬀective surface diﬀusion coeﬃcient vs the chain length N (i.e., the degree of polymerization). Symbols are experimental data, and the solid lines depict the scalings ⟨τdes⟩ ∼ Nβ and Deff ∼ Nγ, where the best-ﬁt exponents are β = 0.6 ± 0.1 and γ = −0.6 ± 0.2, respectively. The error bars are standard deviations from ﬁve random subsets of the data. (c) Scaling of the adsorption rate with chain length, as determined by ﬁtting the experimental displacement distributions with the model for intermittent hopping. The solid line depicts the scaling Qads ∼ Nδ, where δ = −1.2 ± 0.1.

Figure 5. Mean square displacement as a function of time. Symbols are experimental data for PEG of diﬀerent molecular weights (as annotated), and solid lines are least-squares ﬁts to the expression ⟨r2⟩ = 4Γ(Δt)α. The best-ﬁt exponents are α = 1.04(1), 0.98(3), 1.00(5), 0.94(8), and 0.9(1) for the 2, 5, 10, 20, and 40 kg/mol data, respectively. The dashed line illustrates the linear dependence of the MSD on time (i.e., Fickian diﬀusion).

interaction and bulk diﬀusivity.33 Strong adsorption implies that the molecule desorbs and readsorbs many times before it is ﬁnally lost to the bulk. The resulting desorption-mediated steps are power-law-distributed, and the many-step displacement distribution is a Cauchy distribution with power-law tails.25 It should also be noted that the predicted Cauchy distribution holds only over limited time and length scales and transforms into a Gaussian distribution at long times and lengths.25 To compare our experimental results with the standard model for desorption-mediated displacements, in principle one could attempt to ﬁt the tails of the displacement distributions in 1330

dx.doi.org/10.1021/ja407396v | J. Am. Chem. Soc. 2014, 136, 1327−1332

Journal of the American Chemical Society

Article

processes.34,35 A spectrum of binding energies might result from polymer chains having long-lived, nonequilibrium binding conﬁgurations or from chains having a distribution of adsorbed “train” lengths.17,36 A power-law distribution of waiting times was also observed for DNA-coated particles moving on a surface, where the number of particle−surface bonds was a random quantity.35 There are two possible interpretations of the power-law scaling of the mean waiting time (Figure 4a). If all of the adsorbed segments were released at the same time, there would be a single energy barrier to desorption, and the waiting time would have an exponential dependence on the barrier height.37,38 Our simulations suggested that the polymer adsorbed from solution with ∼N0.6 monomers in contact with the surface. If desorption occurred from the same conformation (i.e., if relaxation of the chain on the surface was slow), the desorption energy would have scaled as ∼N0.6, giving rise to a stretched exponential increase in mean waiting time (which might appear similar to a power law over a limited measurement range). The second possibility is that bound segments of the polymer chains desorbed in a step-by-step rather than a concerted manner. When adsorbed chain segments detach sequentially and are kinetically independent of each other, the time for chain detachment has a power-law dependence on the chain length.38 We favor the second interpretation because a desorption mechanism involving sequential, kinetically independent events is also consistent with the power-law waitingtime distributions discussed above. Three-Dimensional Surface Conformations. The scaling exponents we observed (0.6, −0.6, and −1.2) are reminiscent of the so-called Flory exponent for a three-dimensional chain in a good solvent (ν = 0.6); for example, the characteristic size (radius of gyration) of a three-dimensional coiled chain exhibits this same dependence on molecular weight. This suggests that the PEG chains in these experiments, even when in contact with the hydrophobic surface, adopted conformations similar to those expected in bulk solution. In contrast, if the adsorbed chains adopted strictly two-dimensional conformations (pancakes), the number of adsorbed monomers would increase in proportion to N, and the waiting times would fall oﬀ exponentially with chain length rather than as a power law as we observed. That we should ﬁnd behavior appropriate for a three-dimensional chain contrasts with conventional equilibrium models and many experiments that ﬁnd a ﬂattened, two-dimensional conformation for adsorbed polymers.9,39,40 More extended three-dimensional conformations might be the result of weak adsorption or a very slow approach to equilibrium that prevented the chains from ﬂattening onto the surface before they desorbed back into solution.

proportional to Qads. For comparison, a perfectly adsorbing sink of the same strength would have a width r* = D/(Qadsb). On the basis of our above scaling arguments, r* does not have an explicit dependence on molecular weight, suggesting that the timeindependent step size distribution W(r) (eq 1) is also independent of molecular weight. Thus, the diﬀerences between the displacement distributions shown in Figure 2 are governed by diﬀerences in the waiting-time distributions. The invariance of the step-size distribution W(r) with molecular weight is also consistent with the observed scaling of the eﬀective surface diﬀusion coeﬃcient, Deff. If Deff ∼ ⟨W(r)2⟩/ ⟨τdes⟩ and W(r) is constant, then Deff would be expected to scale as the desorption rate ⟨τdes⟩−1; this is precisely what we found by ﬁtting the data in Figure 4 (i.e., Deff ∼ ⟨τdes⟩−1 ∼ N−0.6). This scaling of the surface diﬀusion coeﬃcient with chain length diﬀers from what was found in previous investigations. Conventional theory and simulations of polymer surface diﬀusion (which assume a two-dimensional model for displacements) predict that the surface diﬀusion coeﬃcient should scale as D ∼ N−α with exponents in the range 3/4 < α < 3/2,6−9 but those models do not consider desorption as a mechanism of polymer surface transport. Previous experimental measurements of polymer surface dynamics using ﬂuorescence correlation spectroscopy (FCS) found that the apparent diﬀusion coeﬃcient scaled as N−3/2 or N−1.9,10 The diﬀerence between the scaling exponents in our observations and previous FCS experiments suggests either that there was a fundamentally diﬀerent transport mechanism or that the experimental methods were sensitive to diﬀerent features of the dynamics. FCS measures temporal ﬂuctuations, so it cannot explicitly distinguish between intensity ﬂuctuations that arise from adsorption/desorption events and lateral diﬀusion through a deﬁned focal volume. In the current model, surface diﬀusion and desorption occur via the same temporal process, and our observed distribution of waiting times ψ(τdes) ∼ τdes−(1+α) with α = 1.5 would contribute a decay of ∼τ−1.5 to the ﬂuorescence correlation, similar to the ∼τ−1.0 decay assumed for Gaussian diﬀusion in an FCS experiment. We also cannot rule out the possibility that subtle diﬀerences in the experimental systems used (e.g., long-chain alkane surfaces in which chains might become entangled vs our TMS surfaces) may also result in fundamentally diﬀerent polymer dynamics. In contrast to earlier work that found diﬀerent chain-lengthdependent dynamic regimes,10 we found that a single desorptionmediated mechanism explains all of our experimental data. Over the range of molecular weights studied, there was no apparent transition in the dynamics, for example, from a desorptionmediated mechanism for small chains to an in-plane mechanism for longer chains. Although it is possible that our limited localization precision masked a very slow, in-plane diﬀusive mode (